Sonochemical synthesis of SnS and SnS2 quantum dots from aqueous solutions, and their photo- and sonocatalytic activity

Graphical abstract


Introduction
Sonochemistry is a division of chemistry which studies the overall chemical effects of interaction of ultrasound with investigated system.During the passing of ultrasound wave through liquid a fluctuations of pressure are created what affects the solubility of gases in liquid.This leads to formation of cavitation bubbles which grow through the diffusion into their volume of gases dissolved in liquid.When a bubble reaches its maximum size it collapses generating relatively very high temperatures and pressures of orders of magnitudes 10 4 K and 10 3 atm respectively [1,2].Under such extreme conditions many chemical reactions may occure.One such example is the sonolysis of water forming radicals H ⋅ and ⋅ OH, which is probably the most basic sonochemical reaction [1,2]: Many applications of sonochemistry include synthesis of inorganic materials, which composition may vary from simple (two-element, e.g.ZnS, Bi 2 S 3 ) to complex (many-element, e.g.CuInS 2 , Cu 3 BiS 3 , Cu 2 ZnSnS 4 ) [3][4][5][6][7].They may be obtained in forms varying from nano-to microparticles of diverse morphology.The control of size and shape of synthesized materials may be further improved by merging sono-and electrochemical syntheses [8 -11].The most important thing about the sonochemical synthesis is that it is typically conducted at mild conditions (room temperature, normal pressure) and in many cases it allows using water as a solvent thus avoiding usage of toxic and hazardous organic solvents used in methods such as solvothermal synthesis or hotinjection reaction [2][3][4].Moreover, the application of ultrasound

1. Materials and reagents
All chemicals used in this study were pure for analysis (producer: POCH).For sonochemical syntheses, SnCl 4 ⋅5H 2 O, SnCl 2 ⋅2H 2 O and thioacetamide (TAA) were used as reagents.Distilled water was used as a solvent and ethanol was used for the purification of prepared suspensions.

Sonochemical syntheses and purification of products
The sonochemical syntheses were conducted in conical flasks of mL volume in an ultrasonic cleaner (PS 10A) generating an ultrasound of 40 kHz frequency with nominal power of ultrasounds 60 W. The acoustic power of utilized cleaner was 27.9 W/L according to calorimetric measurements.The procedure for syntheses and purification of obtained powders was adopted from previous Matyszczak et al. investigation [31].
In all syntheses following amounts of reagents were used: 701 mg of SnCl 4 ⋅5H 2 O or 452 mg of SnCl 2 ⋅2H 2 O, 376 mg of thioacetamide, and mL of distilled water as solvent.All reagents were stirred for 10 min with a magnetic stirrer before the start of the reaction.The duration of sonication was 60 and 120 min.After that and before the purification the open conical flasks with obtained powders suspended in original reaction mixture were kept under laboratory hood for 10 min to remove the toxic gases generated during reaction.
The products of syntheses were separated from the reaction mixture by centrifugation.After first centrifugation, a supernatant (reaction mixture) was removed and portion of fresh ethanol was added.Then the powder was suspended in the fresh ethanol by sonication (10 min) and mixing by plastic Pasteur pipette.Then the centrifugation was repeated, supernatant removed, and another portion of fresh ethanol was added.After that, powder was again suspended in fresh ethanol.Then the suspension was centrifuged, supernatant was removed and the powder was finally suspended in another portion of fresh ethanol.

Evaluation of sonochemical efficiency and percentage yield of the synthesis process
The percentage yield and the sonochemical efficiency of the synthesis process were calculated according to the two following equations: Both values (Y and SE) are calculated in reference to the dried products which were obtained by drying of purified suspensions in ethanol under laboratory hood for approximately 3 days.

Uv-vis spectrophotometry (Tauc method)
The UV-Vis spectrum of obtained suspension of product of synthesis in ethanol was collected using UV1600 spectrophotometer (AOE Instruments) and then was used to perform analysis based on the Tauc G. Matyszczak et al.

method:
(αhν) where: αthe linear absorption coefficient (cm − 1 ) hνthe energy of electromagnetic wave (eV) Aconstant E g -the optical energy bandgap (eV) nthe number associated with distinct electron transition type: n = 1 2 for direct allowed transition, n = 3 2 for direct forbidden transition, n = 2 for indirect allowed transition, n = 3 for indirect forbidden transition.

FT-IR investigation
The Fourier-transform infrared spectroscopy measurements were conducted using NICOLET 6700 FT-IR spectrometer.Dried powders of synthesized materials were grounded with KBr and formed as pellets.

Raman spectroscopy investigation
Micro-Raman measurements were conducted using a Renishaw inVia Reflex spectrometer in backscattering geometry.The 633 nm line of the He-Ne-ion laser was used as the excitation.Raman spectra were collected at room temperature and under normal conditions.The spectral resolution of the measured spectra in this configuration was about 1.2 cm − 1 .

XPS investigation
The suspensions of samples were dripped on a conductive tape and left to dry in laboratory fume cupboard.The procedure was repeated until a visible sample layer was obtained then samples were introduced to the spectrometer.X-ray photoelectron spectra (XPS) were recorded by Prevac set-up equipped with high intensity monochromatic X-ray Al Kα (1486.69eV) source Scienta MX 650 (set at 300 W), Scienta R4000 hemispherical analyser, and charge neutralization.The wide spectra were registered with pass energy 500 eV and the step 0.5 eV.The narrow scans were acquired with pass energy 200 eV and the step 0.2 eV for Sn 3d line and step 0.1 for S 2p line.The full width at half maximum (FWHM) for the Au 4f 7/2 line measured at the same experimental condition was equal to 0.6 eV regardless of energy step.The energy scale was calibrated setting the C 1 s line at the position 284.5 eV.Spectra were analysed using the commercial CASA XPS software package (Casa Software Ltd, version 2.3.17)[47] with Shirley background and a GL (30) line shape (70 % Gaussian, 30 % Lorentzian).

SEM investigations
The Scanning Electron Microscopy SEM investigations were performed on the microscope made by Hitachi model SU8000.The powder samples were deposited on carbon tape after drying.The observations were taken at low voltage range between 3 up to 5 kV accelerating voltage.The Secondary Electrons SE were used to register images of surface topography at magnification range of 40 000 times.Fig. 2. Powder X-ray diffractograms diffraction patterns of products of syntheses sonochemically synthesized SnS and SnS 2 quantum dots.

Powder X-ray diffraction
The powder diffraction data were collected for dried samples using X-ray diffractometer Bruker D8 ADVANCE and filtered Cu Kα radiation (λ = 0.154056 nm) at room temperature.The parameters during measurements were as follows: voltage − 40 kV, current -40 mA, angle range from 10 • to 80 • , step Δ2Θ − 0.025 • , counting time -3 s.

HR-TEM and EDX investigations
One drop of the powder suspended in ethanol was deposited on a standard TEM copper grid coated with an amorphous carbon film.After the grid went completely dry it was ready to put into the microscope.
Investigations were conducted on the FEI Titan Cubed 80-300 TEM with an accelerating voltage of 300 kV and the point resolution of 130 pm.The overview images were registered in bright-field TEM mode for magnifications ranging from 9.800x to 55.000x.For the purpose of highresolution imaging magnifications from 145.000x − 380.000x range were used.In both cases, the images were obtained with the Gatan BM-Ultrascan CCD camera.STEM (scanning mode) images were acquired with the use of the HAADF detector which registers strongly scattered electrons.The in situ EDAX spectrometer was used for the analysis of the specimen's elemental composition.

Photo-and sonocatalytic experiments
For degradation experiments we have chosen azo-dye Metanil Yellow which structural formula is displayed in Fig. 1.Despite its high toxicity it is illegally used in food industry especially in India, e.g. as adulterant in turmeric powders [48,49].There are evidences for mutagenic and carcinogenic actions of azo-dyes against human [50][51][52].
Before both photo-and sonocatalytic experiments a 30 mL of dye solution in distilled water was placed in the beaker equipped with magnetic bar.A portion (20 mg) of specific tin sulphide powder was weighed and placed in 5 mL of distilled water and sonicated for 40 min.Such a suspension was then added to the beforehand measured 30 mL of dye solution.To ensure the quantitative transfer of catalyst to the dye solution, the leftovers of catalysts suspension were washed 5 times with 1 mL of distilled water (each time additionally applying sonication for 10 s).Finally the volume of dye solution mixed with the suspension of catalyst was 40 mL.Each volume was measured using the graduated pipette.The prepared mixture was then stirred on magnetic stirrer with speed of 800 rpm under dark conditions for 30 min to ensure the adsorption-desorption equilibrium.After that, the mixture was used in sono-or photocatalytic experiments.
The photocatalytic process was conducted in a initially used glass beaker of 50 mL volume under ambient temperature and pressure.The source of UV radiation was the UV-C lamp (power 72 W).Each time the position of beaker in reference to the UV lamp, as well as the shape and size of beaker, was exactly the same.The UV irradiation lasted 120 min in each photocatalytic experiment.Experiments were conducted under dark conditions.
The sonocatalytic experiments were conducted in falcons (centrifuge tubes) of 14 mL volume.For one experiment a portion of 7 mL of prepared catalysts suspension in dye solution was measured with pipette and placed in each falcon.Four falcons were then placed in ultrasonic bath under dark conditions and sonicated for 120 min.The positions of falcons in ultrasonic bath were precisely controlled and kept the same in each experiment.The level of water in bath was equal to the level of liquid in falcons.
After both kind of processes the mixture was centrifuged (8000 rpm, 8 min) twice to obtain clear dye solution, free of suspended catalyst and ready for absorbance measurement.The absorbance was measured at 440 nm, corresponding to the maximum of absorbance of Metanil Yellow aqueous solution, using UV-Vis spectrophotometer.Each experiment, including blind test, was conducted 4 times.
The color removal during the processes was calculated according to the following straightforward equation: Where:

CR-percentage color removal [%]
A 0 -absorbance of dye solution before sono-or photocatalytic process A E -absorbance of dye solution after sono-or photocatalytic process.

Investigation of synthesis efficiency
Products of syntheses formed uniform suspensions of yellow-orange color (in the case of SnS 2 syntheses) or dark-brown color (in the case of SnS syntheses).Suspensions obtained in the syntheses lasting for 120 min had more intensive colors compared to those obtained in 60 min long reactions, what is undoubtedly caused by formation of greater amount of product under longer sonication.The calculated percentage yields of performed sonochemical syntheses as well as sonochemical efficiencies of formation of SnS and SnS 2 in varying time of synthesis are presented in Table 1.As may be seen, almost full overreaction of SnCl 4 to SnS 2 may be achieved under sonication lasting 120 min while at the same conditions SnCl 2 is converted to SnS in less than 50 %.The calculated values of sonochemical efficiencies show that in reaction lasting 120 min it is possible to obtain c.a. 13 mg of SnS 2 and c.a. 5 mg of SnS in reference to ultrasound of power 1 W. It may be concluded that the sonochemical synthesis of SnS 2 is more efficient than sonochemical synthesis of SnS.

X-ray powder diffraction investigations
The X-ray powder diffraction investigations confirmed the presence of both compounds, SnS and SnS 2 , in nanocrystalline forms as indicated by presence of wide reflexes in the diffraction patterns (Fig. 2).The absence of wide, large peak at the beginning of diffraction pattern suggests that prepared samples are rather nanocrystalline than nanoamorphous.Products of longer syntheses (120 or 90 min) have generally more and/or better shaped reflexes than products of syntheses lasting 60 min.This is apparently due to the greater amount of products after longer sonication.Also, in the case of SnS obtained after 90 and 120 min of sonication more reflexes are present what may be linked to better crystallinity of sample.

FT-IR investigations
The Fourier transform infrared spectroscopy investigation confirms the presence of tin sulphides in prepared samples.The corresponding spectra are presented in Figure S1.They show the occurrence of trace amounts of solvents used in syntheses (H 2 O) and purification (C 2 H 5 OH) as indicated by peaks corresponding to C-C and C-H bonds, and -OH groups.The bands related to Sn-S bond are similar in both samples of SnS 2 what is in line with the XRD result.However, significant difference is observed between spectra of SnS obtained after 60 and 120 min of sonication.In the latter case the band is much more defined revealing that the product of longer synthesis is of better crystallinity.This result is also in line with the XRD result.

Raman spectroscopy investigations
The Raman studies were performed to investigate the microstructural phase homogeneity of the sulphide samples.The studies have shown that the investigated samples are homogeneous in terms of chemical composition.For products of sonochemical syntheses of SnS 2 the recorded spectra corresponded to the rhombohedral structure of SnS 2 .This is evidenced by a clear peak of A 1g symmetry for about 315 cm − 1 (Fig. 3, on the left) [53,54].In the case of SnS 2 obtained under sonication lasting 60 min, for a few measurements, a slight shift of this peak towards lower frequencies was observed.This shows that we are dealing with different polytypes of the SnS 2 structure [55].Some asymmetry was also observed for the 315 cm − 1 peak.As a rule, such asymmetry occurs when phonons interact with free carriers or is the result of phonon constraints in nanostructures [56,57].The low excitation energy used in the Raman studies (633 nm) in relation to the width of the SnS 2 energy gap allows excluding the interference factor between phonons and electrons from the conduction band.The asymmetry of the peak should therefore be interpreted as an effect of the small size of SnS 2 grains and the resulting phenomena of quantum confinement.
In the case of products of sonochemical syntheses of SnS, the spectrum corresponds to that recorded for SnS nano grains [53,58].Both peaks present in the spectra for about 225 cm − 1 and about 305 cm − 1   (Fig. 3, on the right) are rather present in poorly crystallized SnS nano grains.In the case of nanostructures with SnS stoichiometry, the literature data shows the presence of both peaks, for 225 cm − 1 and for about 305 cm − 1 [58].The peak at 225 cm − 1 comes from interatomic vibration between metal (Sn) and chalcogen (S).With the advancing crystallization process, the peak at about 190 cm − 1 [53] becomes dominant for bulk samples of SnS, which was not observed in the tested samples.At the same time, in crystalline bulk samples of SnS, the peak for about 305 cm − 1 disappears.The peak at about 305 cm − 1 can also be interpreted as the presence of the Sn 2 S 3 phase, especially since for some grains only a wide peak at 305 cm − 1 was recorded (spectrum 120 min-02-Sn 2 S 3 , Fig. 3, right).For Sn 2 S 3 structure the peak at 305 cm − 1 is associated with the intralayer vibration of chalcogen-chalcogen ions [58].G. Matyszczak et al.

Scanning electron microscopy investigations
Scanning electron microscopy observations were used to study the morphology of synthesized tin sulphides (Fig. 4).The dried powder of SnS 2 synthesized under sonication lasting 60 min shows a bit rough surface without any characteristic particles.In the case of SnS 2 synthesis with duration of 90 and 120 min, the dried product had wavy surface, and very small particles with size smaller than 0.1 μm (100 nm) may be observed.SEM images of SnS powders reveal the presence of rather uniform particles of granular shape and submicron size.SnS powder synthesized with longer sonication time exhibited larger particles.EDX measurements confirmed the elemental composition of SnS and SnS 2 samples.Relevant Sn:S atomic ratios are nearly 1:1 for SnS and 1:2 for SnS 2 samples.

High-resolution transmission electron microscopy investigations
The high-resolution transmission electron microscopy observations of SnS samples obtained sonochemically reveal the presence of nanocrystallites of size lying in approximate range 3-8 nm for 60 min of sonication.For SnS powders obtained after 90 min of sonication two types of entities could be observed.Generally they formed either polycrystalline clusters with mostly indistinguishable grain boundaries (the ones that could be distinguished have sizes in range 3.5 -7.5 nm) or longitudinal nanocrystals being max.40-50 nm long with width not exceeding 5 nm.In the case of SnS powder synthesized under 120 min of sonication nanoparticles of two kinds were observed: one had sizes in range c.a. 3 -7 nm and the others had sizes in range c.a. 30---40 nm.However, in the case of sonochemical synthesis of SnS 2 , the nanoparticles had sizes lying in range c.a. 1.5 -3.5 nm independently from the duration of synthesis.SnS 2 sample obtained after 90 min of reaction also appeared to be a highly polycrystalline material and most grain boundaries in this case were also difficult to distinguish.In this case, also larger crystallites were observed (i.e. with sizes in range 5 -10 nm).Generally, synthesized in this study SnS 2 nanoparticles were smaller than the SnS nanoparticles (Fig. 5).
Fourier transform analysis of HR-TEM images of SnS particles obtained under sonication lasting 60 min showed that they fit to the orthorombic primitive structure of two possible space groups -Pnma of cell parameters a = 11.201( 5 (the crystallite is oriented in [2 3 1] direction) -see Fig. 6.The same kind of agreement was also observed for SnS sample obtained after 90 min of sonication.In this case values of interplanar spacings obtained based on Fourier transform analysis also fitted the same two orthorombic primitive structures of SnS (Pnma with crystallite seen in [0 0 1] zone axis and Pmcn with crystallite seen in [0 1 0] zone axis).The same was observed for SnS particle in powder obtained under sonication lasting 120 min with the difference that the directions were [1 0 1] and [0 1 1] for Pnma and Pmcn space groups respectively.Fig. 6 presents similar structural analyses, based on HR-TEM images, also for SnS 2 obtained sonochemically.In the case of product of synthesis lasting 60 min analysis of nanoparticle of dimensions c.a. 3.2 x 2.0 nm revealed that it fits a trigonal primitive structure of SnS 2 with space group P-3 m1 of cell parameters a = b = 3.638(3) Å, c = 5.88(1) Å, α = β = 90 • , γ = 120 • .The crystallite is seen in [1 2 2] direction.As mentioned earlier, the SnS 2 powder obtained after 90 min of reaction is highly polycrystalline and for this sample it was not possible to find single crystallites with a clearly visible atomic arrangement to analyze it in a similar manner as in previous cases.Fourier transform analysis from a whole HR-TEM image allowed to determine four characteristic interplanar spacings which match the spacings of two hexagonal primitive structures (P-3 m1 (ICSD # 100610) -d 110, 1-20 = 0.182 nm, d 011 = 0.278 nm, d 010 = 0.315 nm and d 001 = 0.588 nm and P6 3 mc (ICSD # 43003) -d 110, 1-20 = 0.182 nm, d 012, 1-12 = 0.278 nm, d 010 = 0.315 nm and d 002 = 0.591 nm).Interestingly, for this sample single nanocrystals (with sizes in range 3-10 nm, see Fig. 5) with one specific atomic plane could be observed.Its interplanar distance equals 0.59 nm and it's one of the four characteristic distances measured for the polycrystalline material.As mentioned above, this value corresponds to the {0 0 1} planes of the hexagonal primitive structure with P-3 m1 space group or the {0 0 2} planes of hexagonal primitive structure with P6 3 mc space group.In the case of SnS 2 synthesized under 120 min of sonication a nanoparticle of dimensions c.a. 2.5 x 3.5 nm was analyzed.It also fits a trigonal primitive structure of space group P-3 m1.The crystallite is oriented in [0 1 1] direction.
The calculations performed using the Scherrer equation for SnS samples, taking K = 0.9 and.λ = 0.154056 nm, gave following values of crystallites mean sizes: 4.5 nm (60 min long synthesis), 6.2 nm (90 min long synthesis), and 6.4 nm (120 min long synthesis).These values are in good agreement with the HR-TEM observations.For SnS 2 samples such calculations weren't possible due to insufficient quality of powder diffractograms for this samples.
It is postulated that the sulphides are formed via precipitation due to the formation of hydrogen sulfide formed in the hydrolysis of thioacetamide: Taking into account that the size of nanocrystallites is rather similar towards different synthesis times, it is postulated that the main mechanism of growth of nanoparticles is the precipitation mechanism and, once formed, the nanoparticles do not expand significantly.

X-ray photoelectron spectroscopy
The concentration of main elements was estimated from high resolution XPS spectra and collected in Table 2.The presence of tin, sulfur as well as carbon and oxygen was found on the surface of the tested samples.At the level of few percentage nitrogen and chlorine were also detected in wide spectra.As they come from technological process they were not considered in analysis.
The analysis of Sn 3d5/2 and S 2p lines (Figs. 7-8 and Table 3) was focused on the evaluation of the chemical states of Sn and S in the studied samples.The XPS survey scans are provided in supplemental materials as Figures S2-S6.In Table 3 the binding energy and the full width at half maximum (FWHM) of given component is collected.The binding energy (BE) of Sn(II) 3d5/2 line in SnS (BE = 486.0eV) is about 1 eV smaller than Sn(IV) in SnS 2 (BE = 487.0eV) [59].For Sn(0) BE = Table 3 The binding energy (eV); percentage of given fraction, and full width at half maximum (eV) (FWHM) for chemical components in analysed samples.FWHM indicates the level of chemical order in formed compounds.484.8 eV was reported [60].Moreover, the BE of Sn in oxides is very similar to that in sulphides [60].Therefore, if the content of Sn and S differs from stoichiometry of SnS and SnS 2 , which is observed for both SnS 2 samples and SnS (120 min) nanoparticles (see Table 2), we can assume that excess of Sn is bonded with oxygen.The chemical shift between S 2p3/2 bonded in SnS (BE = 160.9eV) and in SnS 2 (BE = 162.1 eV) is also close to 1 eV.From Table 3 one can see that only for sample SnS 2 (60 min) one component was formed with quite narrow lines.For all other samples we found two components in different proportions.In sample SnS 2 (120 min) 9 % of S was bonded in SnS form and in SnS (60 min) still 17.6 % S was in SnS 2 form.Moreover, for SnS (90 min) all sulphur was in SnS 2 and for SnS (120 min) most of the sulphur was in SnS 2 form.

Determination of energy bandgap value using Tauc method
The results of analyses based on Tauc method show that synthesized samples differ greatly in value of direct optical energy bandgap (Fig. 9).Corresponding absorption spectra are provided in the supplemental materials as Figures S7 and S8.SnS quantum dots have direct energy bandgap of value 2.31 eV, 1.47 eV and 1.05 eV for products of synthesis lasting 60, 90 and 120 min respectively.On the other hand, SnS 2 quantum dots have direct energy bandgap of value 2.88 eV, 2.78 eV and 2.70 eV for products of synthesis lasting 60, 90 and 120 min respectively.In the case of SnS, the difference between samples is significant, in contrast to the case of samples of SnS 2 .The referential, literature values of bandgaps for bulk SnS and SnS 2 are 1.32 eV and 2.38 eV respectively [22,61,62].Quantum dots of SnS obtained under sonication

Sonocatalytic and photocatalytic activity
Each obtained nanopowder was applied as catalyst in the photo-and sonodegradation of azo-dye Metanil Yellow.The values of mean percentage color removal, CR, for each of investigated tin sulphide quantum dots and for each process were presented on Fig. 10.The greatest color removal was observed in the sonocatalytic degradation applying SnS quantum dots, synthesized through sonication lasting 120 min, as catalyst (85.2 % color removal).Overall, the sonocatalytic process was more efficient than the photocatalytic one.However, exceptions were observed when as catalyst quantum dots of SnS 2 prepared in synthesis lasting 90 and 120 min were used.In these cases the photocatalytic process showed, respectively, 62.0 % and 66.9 % color removal while in the sonocatalytic process the removal was, respectively, 39.3 % and 38 % only.Quantum dots of SnS 2 obtained under sonication lasting 120 min were the best photocatalyst, while quantum dots of SnS obtained under similar sonication time were the best sonocatalyst.The worst catalyst, in both sono-and photocatalytic degradation (color removal 19.5 % and 13.2 % respectively), were quantum dots of SnS 2 obtained in synthesis lasting 60 min.Additionally, it may be seen from Fig. 10 that prepared SnS quantum dots exhibited in both the photo-and sonocatalytic activity for powder prepared under sonication lasting 90 min.
The photocatalytic process depends on the absorption of incident photon by the catalyst thus the activity of catalyst should depend on the value of optical energy bandgap.In this study, the best photocatalyst had bandgap of 2.70 eV value, however there is no explicit dependence between photocatalytic activity and optical bandgap among tested samples.This is clearly shown in the case when SnS quantum dots where applied as photocatalyststhey differed much in value of optical bandgap (2.31 eV and 1.05 eV) but exhibited similar color removal under the same conditions.Despite the fact that for the SnS 2 samples the longer the synthesis time the lower the energy bandgap, there must be additional factor that affects the photocatalytic activity.On the other hand, the sonocatalytic process consists of three main effects: promotion of acoustic cavitation, photoexcitation by light generated by sonoluminescence, and thermal excitation by heat generated from collapse of acoustic bubbles [44].Many parameters affect each of these three mechanisms: the value of optical bandgap should affect the photoexcitation, shape and sizes of particles of catalyst should affect the ability for promotion of ultrasonic cavitation and thereby these parameters should also affect the thermal excitation (more acoustic cavitation = more heat generated), also the ability to thermal excitation depends on kind of material of which catalyst is made.The detailed mechanisms of photoand sonocatalytic processes should be more investigated (in general) to let explain the differences among tested samples of nano tin sulphides.In our study there is no clear correlation between crystallite sizes, optical energy bandgap, and chemical states (Sn(II)/Sn(IV) on the surface of nanoparticles) on the catalytic activity.Probably the observed differences in photo-and sonocatalytic activities is caused by complex interplay of these factors.

Conclusions
We synthesized quantum dots of SnS and SnS 2 in sonochemical synthesis using water as a solvent and thioacetamide as sulfur source.We provided values of the sonochemical efficiencies of nano tin sulphides syntheses under distinct sonication times what allows for scaling up of the process.Generally, the syntheses of SnS 2 quantum dots were more energetically efficient than the syntheses of SnS quantum dots as sonochemical efficiencies for syntheses lasting 120 min were of values 12.98 mg/W and 4.97 mg/W, respectively.Performed characterization of products of syntheses confirmed the desired composition of samples (SnS and SnS 2 ) and proved that products of syntheses consists of quantum dots of typical sizes in range 3-8 nm for SnS and 1.5 -10 nm for SnS 2 .In the case of synthesis of SnS lasting 90 and 120 min also larger nanoparticles, of sizes in range 30---50 nm, were observed.Raman studies confirmed the structural homogeneity of products of syntheses of which the desired product was tin(IV) sulphide.Each sample had a SnS 2 structure.On the other hand, products of syntheses of which the desired product was tin(II) sulphide had characteristic modes for SnS nano grains.The peak at 305 cm − 1 in these samples can be interpreted as the presence of traces of the Sn 2 S 3 phase.XPS investigation proved that nanoparticles contain tin mainly on desired oxidation state (Sn(II) for SnS and Sn(IV) for SnS 2 ).Exception was observed in the case of nano-SnS synthesized under sonication lasting 90 and 120 min, where on the surface of nanoparticles tin is present in both oxidation states with higher amount of Sn(IV).Moreover, substantial part of Sn in this sample is bonded to oxygen.According to the results of analysis performed with the Tauc method, SnS quantum dots have direct energy bandgap of value 2.31 eV (60 min of synthesis), 1.47 eV (90 min of synthesis), and 1.05 eV (120 min of synthesis).On the other hand, SnS 2 quantum dots have direct energy bandgap of value 2.88 eV (60 min of synthesis), 2.78 eV (90 min of synthesis), and 2.70 eV (120 min of synthesis).These observations are mainly caused by the quantum confinement effect.The comparison of percentage color removal in the photo-and sonocatalytic degradation of azo-dye Metanil Yellow using synthesized quantum dots as catalysts shows that the most efficient sonocatalyst was nano-SnS obtained in sonochemical synthesis lasting 120 min (85.2 % color removal).On the other hand, the most efficient photocatalyst was nano-SnS 2 obtained applying the same time of synthesis (66.9 % color removal).

Fig. 6 .
Fig. 6.Structural analyses of SnS and SnS 2 nanoparticles obtained under distinct sonication times, based on HR-TEM images.

Fig. 10 .
Fig. 10.Values of mean percentage color removal for sonochemically synthesized quantum dots of SnS and SnS 2 under varied sonication time, in two different degradation processes: photo-and sonocatalytic.

Table 1
Percentage yields and sonochemical efficiencies of performed syntheses.

Table 2
Results of the XPS and EDS elemental composition (at %) of tested samples from high resolution spectra.